Carrier multiplication detected through transient ... - Nature › publication › fulltext › Carrier-m... › publication › fulltext › Carrier-m...by J Gao · 2015 · Cited by 46 — and also provide new insights into effects of electric field and ligand treatment
Carrier multiplication detected through transient photocurrent in device-grade ﬁlms of lead selenide quantum dots Jianbo Gao1,w, Andrew F. Fidler1 & Victor I. Klimov1
In carrier multiplication, the absorption of a single photon results in two or more electron–hole pairs. Quantum dots are promising materials for implementing carrier multiplication principles in real-life technologies. So far, however, most of research in this area has focused on optical studies of solution samples with yet to be proven relevance to practical devices. Here we report ultrafast electro-optical studies of device-grade ﬁlms of electronically coupled quantum dots that allow us to observe multiplication directly in the photocurrent. Our studies help rationalize previous results from both optical spectroscopy and steady-state photocurrent measurements and also provide new insights into effects of electric ﬁeld and ligand treatments on multiexciton yields. Importantly, we demonstrate that using appropriate chemical treatments of the ﬁlms, extra charges produced by carrier multiplication can be extracted from the quantum dots before they are lost to Auger recombination and hence can contribute to photocurrent of practical devices.
for Advanced Solar Photophysics, Chemistry Division, Los Alamos National Laboratory, Los Alamos, New Mexico 87545, USA. w Present Address: Chemistry Department, University of California, Berkeley, California 94720, USA. Correspondence and requests for materials should be addressed to J.G. (email: [email protected]
) or to V.I.K. (email: [email protected]
NATURE COMMUNICATIONS | 6:8185 | DOI: 10.1038/ncomms9185 | www.nature.com/naturecommunications
& 2015 Macmillan Publishers Limited. All rights reserved.
NATURE COMMUNICATIONS | DOI: 10.1038/ncomms9185
rocesses of photon-to-charge-carrier conversion are of key importance in photosynthesis, generation of solar fuels, and production of photoelectricity. A traditional assumption is that a single photon is converted into a single electron–hole (e–h) pair or an exciton. However, the fundamental laws of physics do not prohibit the absorption of a single photon from producing multiple e–h pairs if the photon energy (hv) is sufﬁciently high to ensure energy conservation. This process, usually termed ‘carrier multiplication’ (CM) or ‘multiexciton generation’, can be understood in terms of impact ionization whereby a valence band electron is promoted across a band gap (Eg) as a result of a collision with an energetic carrier (an electron or hole) (Fig. 1a). Ideally, quantum efﬁciency (QE) of photon-toexciton conversion (q) in the presence of CM is characterized by a staircase-like function where each increment of hv by Eg results in a new e–h pair, that is, an increase in QE by 100% (Fig. 1b; blue line). If CM operates at this energy-conservation deﬁned limit, it could lead to dramatic advances in solar energy conversion technologies1,2. In macroscopic, ‘bulk’ semiconductors, however, CM is inefﬁcient within the solar spectrum due to a high activation threshold (ECM) which is at least B4Eg (refs 3,4) (Fig. 1b; red line). As was originally demonstrated in ref. 5 the CM threshold could be considerably reduced (to o3Eg) using nanosized semiconductor crystals known as quantum dots (QDs), and further pushed down to the fundamental 2Eg limit through QD hetero-structuring6 (Fig. 1b; green line). The observed reduction in ECM can be linked to relaxation of constrains imposed by translation momentum conservation due to suppression of translation motion of carriers in QDs7–9. In addition, CM in QDs beneﬁts from a discrete, atomic-like structure of electronic states, which makes a competing process of photon emission less efﬁcient than in the bulk2. Following the original report on CM in PbSe QDs5, this process has been observed in QDs of a variety of compositions5,10–15, as well as other nanomaterials including semiconductor nanorods16, semiconductor heterostructures6,17, carbon nanotubes18 and graphene19. Considerable progress has also been made towards demonstrating CMenhanced photocurrent in practical devices20–22 as well as the development of various theoretical frameworks for treating this process in nanomaterials8,23–28. While the conducted studies have indicated a signiﬁcant promise of engineered nanostructures for obtaining enhanced CM, there are still a number of questions and challenges that need to be addressed to fully realize the potential of CM in practical devices. For example, the majority of quantitative insights into
CM has been derived from optical spectroscopic studies of solutions of isolated QDs29–31, while practical devices use ﬁlms of electronically coupled particles20,22,32–35. The available studies of QD ﬁlms, however, do not provide a conclusive answer to the question on the effect of electronic coupling on multiexciton yields. For example, time-resolved microwave conductivity measurements indicate that CM efﬁciencies in PbSe QD ﬁlms can be considerably higher than those in QD solutions36. On the